Nanosize CaCu3Ti4O12 Green Synthesis and Characterization of a Precursor Oxalate Obtained from Averrhoa carambola Fruit Juice and Its Thermal Decomposition to the Perovskite

Improving on the very high temperatures used in solid-state synthesis routes to prepare CCTO ignited the idea of using oxalate routes which make use of organic solvents in the synthesis of CCTOX as oxalate intermediates to the decomposition product, CCTO. The use of commercial oxalic acids and oxalate has not only recorded a solubility problem which reflects on the size, shape, homogeneity, and morphology of the final product but also has an environmental impact originating from the solvents used. Both the composition and morphology of these inhomogeneities play a role in the behaviour of the final product, pointing out the need to assess the dependence of size, shape, homogeneity, and morphology and the material performance on the sample synthesis history. In this study, nanosized particles of calcium copper titanium oxide, CaCu3Ti4O12 (CCTO), were successfully synthesized by pyrolysis of the corresponding heterometal oxalate precursors obtained via coprecipitation using the edible carambola fruit juice as a precipitating agent and investigated in detail. The precursors were characterized, and the results revealed the formation of a single molecular precursor represented by the formula CaCu3(TiO)4(C2O4)8·9H2O (CCTOX). The decomposition products, obtained via calcination in air, were subsequently subjected to thermal treatments at different temperatures for 4 hours. The morphology and microstructure were characterized, and analysis showed the formation of a single phase, CaCu3Ti4O12 (CCTO) with CuO and CaTiO3 as impurity. It was observed from microscopy that the samples obtained from sintering at 600C for four hours had discrete particles with regular morphology, limited size distribution, high degree of homogeneity, and multiple dimensions ranging between 10 and 35 nm and showed some degree of ellipticity in shape. Increasing the sintering temperature from 600C to 700C and 800C increased the grain growth in the ceramic as well as the densification. The method makes advantage of the fact that oxalate precursors decomposed at relatively lower temperatures and the fact that the oxalate in the juice is in the solution which downplays both the solubility and environmental pollution problems since no additional solvents are used.


Introduction
Miniaturization of electronic devices with giant dielectric constants is a challenge in in microelectronics. Oxides of the type CaCu 3 Ti 4 O 12 (CCTO) have received research interest because of their very high dielectric constant at room tem-perature, which is around 10 4 to 10 5 at 1 kHz and good temperature stability in a wide temperature range from 100 to 600 K [1]. The cause of this exceptionally high dielectric constant is still debatable, though it has been attributed to grain boundary capacitance and extrinsic defects rather than to the intrinsic properties that result from the crystalline structure of the material [2]. This dielectric material has been shown in multifunctional fields, such as electroceramic, electronic, and microwave devices such as capacitors, gas sensors, and varistors [3,4].
CCTO has a perovskite-like structure derived from the cubic perovskite (ABO 3 ) by an octahedral tilt distortion caused by size mismatch and the nature of the A-site. The size difference between the Ca 2+ and Cu 2+ ions causes the TiO 6 octahedral to produce a structure where threequarters of the sites have square-planar coordination and are occupied by Jahn-Teller distorted Cu 2+ ions [1]. The synthesis methods has control over the particle size, phase purity, and morphology which themselves have a great deal to contribute to material properties and applications, and various methods for the synthesis of CCTO have been reported. The conventional solid-state reaction between stoichiometric starting materials of CaCO 3 , TiO 2 , and CuO followed by calcination at high temperatures (1000-1050°C) for prolonged periods (24-48 hours) has widely been used for synthesizing CCTO [1,5]. This method is very cumbersome with the final product not only containing impurities (secondary phases and unreacted components) but also poor powder characteristics, represented by a coarse particle size, wide particle size distribution, irregular particle morphology, and a high degree of inhomogeneity [6].
Other methods used to synthesize CCTO in literature include microwave heating [7], sol-gel method [3,8], wetchemical method [9], pyrolysis [9], coprecipitation [10], and polymeric precursor route [11]. Pyrolysis has the disadvantage of involving the handling of chemicals in a glove box and refluxing solutions. The sol-gel process uses metal alkoxides as the starting materials, which are costly and extremely sensitive to the atmospheric conditions such as moisture, light, and heat. In contrast, wet chemistry methods afford intimate and homogeneous mixing of the metal ions in stoichiometric ratios at the atomic scale. Pure samples at the nanometer scale could be obtained at lower temperatures and shorter reaction times than that resulting from solidstate reactions. CCTO has also been obtained by the pyrolysis of coprecipitated oxalate at high temperatures (>950°C) for 10 hours. The CCTO obtained had CaTiO 3 + CuO as the impurity phase [12]. The phase purity was only achieved after sintering the powder at 1050°C. It has been observed that the physical properties such as particle size and shape as well as the dielectric properties highly depend on the synthesis technique. The best dielectric properties were shown by the ceramics prepared via the solid-state route despite the high temperature used, while using wet chemistry method is a better approach to obtain a homogeneous and controlled microstructure. A new trend in this area should be in the direction of finding new synthesis methods able to give a homogenous micro-or nanostructure. Such techniques could help reduce the synthesis temperature and achieve high permittivity.
We are reporting an environmentally friendly, facile, cost-effective, and green synthesis method for the synthesis of calcium copper titanate oxalate precursor and its subsequent thermal decomposition at relatively low temperatures and sintering time to CCTO. We use a naturally available resource (Averrhoa carambola L. fruit juice) rather than the commercial sources for the synthesis of metal oxalates. The use of this natural renewable resource is of environmental significance and, in the case of free oxalic acid rich fruits (e.g., Averrhoa carambola L.), could result in a significant reduction in the level of the free acid, thus adding value to the elimination of toxic components through reaction with metal ions. This could also open up the possibility of high value exploitation of spoiled fruits.
Averrhoa carambola, known as carambola or star fruit, is an attractive, exotic, tropical, and shrub-like ornamental tree of the Oxalidaceae family [13]. It is an excellent source of oxalic acid, with oxalic acid contents that can be as high as 1 wt. % of wet mass (representing about 74% of the total acid content depending on the level of maturity of the fruits) [14].
In this paper, we present a facile and green approach for the synthesis of the mixed metal copper titanate oxalate precursor. Our approach is based on coprecipitation of the mixed metal ion solution and the fruit juice extract without the use of hazardous organic compounds or surfactants.

2.2.
Processing of the Fruit Juice. Ripe carambola fruits were harvested, washed under running tap water, and crushed in a blender. The juice was extracted by squeezing through cheese cloth. The collected juice was centrifuged for 20 mins at 3000 rpm, the supernatant was filtered, and the filtrate was collected which was previously characterized [15] and was kept in a freezer for further use.

Synthesis of the Oxalate Precursor.
A solution (0.06 M) of calcium copper titanium composite metal chloride ion was prepared by dissolving the various metal ion chlorides in distilled water. The chlorides were divided into two different solutions. The first one contained stoichiometric amount of calcium chloride and copper (ii) chloride (hydrate) in 200 mL of distilled water, and the second contained stoichiometric amounts of TiCl 3 . This procedure allows obtaining two limpid solutions without the apparition of either a precipitate or gel. 100 mL of the juice extract was poured into a 250 mL round bottom flask immersed into a water bath maintained at 80°C. 50 mL, from each of the chloride solutions, was simultaneously added onto the juice while stirring. The mixture was further stirred for 1 hour. The slurry was allowed to cool at room temperature then aged for 8 hours. The precipitate obtained was filtered, washed several times with distilled water, then ethanol, and oven dried at 100°C for 1 hour.

Thermal Decomposition of the Complexes.
A sample of the dry precursor (0.5 g) was ground and placed in a ceramic crucible, and the crucible placed in the furnace systematically heated to 550°C where a constancy of mass was observed. On 2 Journal of Nanomaterials the other hand, the crucible was placed in the furnace that had been preheated to the desired sintering temperature of 600°C, 700°C, and 800°C and sintered in air continued for 4 h. The sample in each situation was allowed to cool down at room temperature in the furnace. The residues for systematic and isothermal decomposition, respectively, obtained were weighed and kept for further analysis. They represent, respectively, 48.1% and 45.56% of the precursors.

Characterization
Techniques. FT-IR spectra were recorded from 4000 to 400 cm -1 on a PerkinElmer Spectrum on two universal attenuated total reflectance Fouriertransform infrared (UATR-FT-IR) spectrometers. Thermogravimetric analysis (TGA) was obtained using a Pyris 6 Per-kinElmer TGA 4000 thermal analyser. The TGA analysis was conducted between 30°C and 900°C under nitrogen atmosphere at a flow rate of 20 mL/min and a temperature ramp of 10°C/min. The XRD diffractograms of the precursors and the decomposition products were recorded on a Bruker D8 Advance X-ray diffractometer using a Cu Kα radiation source (λ = 0:15406 nm, 40 kV, and 40 mA). Scans were taken over the 2θ range from 10°to 100°in steps of 0.

Thermal Analysis.
A verification of the thermal behaviour of CCT-OX was carried out by thermal analysis (TGA). The TGA/DTG graph of the complex is shown in Figure 2, where four weight loss portions were observed. The complex decomposed to a residue of approximately 48.1% of the original weight (juice complex) at 600°C to a relatively stable intermediate which finally decomposed to the final product after sintering at the decomposition temperature for four hours. This final stage revealed a further weight loss of 2.54% which compares with 45.41% residue (CaCu 3-Ti 4 O 12 ) expected from the decomposition of CaCu 3 (TiO) 4 (-C 2 O 4 ) 8 ·9H 2 O. This pattern agrees with some minute differences with that proposed in literature [15]. The first weight loss (18.1%) corresponds to the elimination of nine molecules of water and two molecules of carbon dioxide (18.4%) giving birth to CaCu 3 (TiO) 4 Figure 4: EDAX elemental composition for the decomposed product (CCTO). 5 Journal of Nanomaterials 3.5. EDS of the Decomposition Product of CCTOX. The representative EDS spectrum for the composition are shown in Figure 4 and integrated with the metal content and elemental compositions. The results indicate the presence of peaks at 0.8 KeV for Ca, 4.5 KeV to 5 KeV for Ti, and 8 KeV to 9 KeV for Cu and reveal a large extent that only copper, calcium, titanium, and oxygen were present in the matrix which confirmed the elemental purity of the constituent atoms in the microstructure of the prepared powders sintered at 600°C for four hours. Empirical formula calculations based on elemental composition, indicated nonstoichiometry in titanium and copper, which can be attributed to the presence of CaTiO 3 and CuO in the microstructure of the CCTO.
3.6. Morphology of the Decomposed Powders (SEM and TEM). The morphology and particle size distributions of the decomposed sample are presented on Figure 5. SEM results showed particles which are weakly agglomerated but whose level of agglomeration increased with the increase in sintering temperature, while TEM images of the obtained ceramic showed a dense microstructure with an average grain size 17 nm. The powders obtained from sintering at 600°C for four hours had discrete particles with regular morphology, limited size distribution, and high degree of homogeneity. The particles show some degree of ellipticity in shape and multiple dimensions ranging between 10 and 35 nm. Increasing the sintering temperature from 600°C to 700°C resulted in densification and increase in the grain growth within the ceramic.

Conclusion
Averrhoa carambola fruit juice has been used as a precipitating agent in the synthesis by coprecipitation of a single molecular precursor CCTOX (CaCu 3 (TiO) 4 (C 2 O 4 ) 8 ·9H 2 O)) which decomposed at relatively low temperature to CCTO (CaCu 3 Ti 4 O 11 (CO 3 )). The technique is simple and environmentally friendly and does not require costly equipment, stringent reactions, or complex procedures yet produced excellent results (phase singular nanosized CaCu 3 Ti 4 O 12 particles which have a regular morphology, limited size distribution, high degree of homogeneity, some degree of ellipticity in shape, and multiple dimensions ranging between 10 and 35 nm) at low decomposition temperature of 600°C and sintering period of four hours.

Data Availability
The datasets used and/or analyzed during the current study are available from the corresponding author upon reasonable request.